Indentation-induced interface delamination of a strong film on a ductile substrate
Thin Solid Films 381 Ž2001. 143 154 Indentation-induced interface delamination of a strong ﬁlm on a ductile substrate A. Abdul-Baqi, E. Van der GiessenU Delft Uni¨ ersity of Technology, Koiter Institute Delft, Mekelweg 2, 2628 CD Delft, The Netherlands Received 15 January 2000; received in revised form 12 July 2000; accepted 12 July 2000Abstract The objective of this work is to study indentation-induced delamination of a strong ﬁlm from a ductile substrate. To this end,spherical indentation of an elastic perfectly plastic substrate coated by an elastic thin ﬁlm is simulated, with the interface beingmodeled by means of a cohesive surface. The constitutive law of the cohesive surface includes a coupled description of normaland tangential failure. Cracking of the coating itself is not included and residual stresses are ignored. Delamination initiation andgrowth are analyzed for several interfacial strengths and properties of the substrate. It is found that delamination occurs in atangential mode rather than a normal one and is initiated at two to three times the contact radius. It is also demonstrated thatthe higher the interfacial strength, the higher the initial speed of propagation of the delamination and the lower the steady statespeed. Indentation load vs. depth curves are obtained where, for relatively strong interfaces, the delamination initiation isimprinted on this curve as a kink. 2001 Elsevier Science B.V. All rights reserved.Keywords: Adhesion; Coatings; Hardness; Interfaces1. Introduction w1x on the ability of using indentation to determine the properties of thin ﬁlms, Swain and Mencik w2x have ˇ Indentation is one of the traditional methods to considered the possibility to extract the interfacial en-quantify the mechanical properties of materials and ergy from indentation tests. Assuming the use of aduring the last decades it has also been advocated as a small spherical indenter, they identiﬁed ﬁve differenttool to characterize the properties of thin ﬁlms or classes of interfacial failure, depending on the relativecoatings. At the same time, for example for hard wear- properties of ﬁlm and substrate Žhardrbrittle vs. duc-resistant coatings, indentation can be viewed as an tile., and the quality of the adhesion. Except for elasticelementary step of concentrated loading. For these complaint ﬁlms, they envisioned that plastic deforma-reasons, many experimental as well as theoretical stud- tion plays an important role when indentation is con-ies have been devoted to indentation of coated systems tinued until interface failure. As emphasized further byduring recent years. Bagchi and Evans w3x, this makes the deduction of the Proceeding from a review by Page and Hainsworth interface energy from global indentation load vs. depth curves a complex matter. U Viable procedures to extract the interfacial energy Corresponding author. Tel.: q31-15-278-65002150; fax: q31-15- will depend strongly on the precise mechanisms in-278-2150. E-mail address: email@example.com ŽE. Van der volved during indentation. In the case of ductile ﬁlmsGiessen.. on a hard substrate, coating delamination is coupled to0040-6090r01r$ - see front matter 2001 Elsevier Science B.V. All rights reserved.PII: S 0 0 4 0 - 6 0 9 0 Ž 0 0 . 0 1 3 4 4 - 4
144 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154plastic expansion of the ﬁlm with the driving force fordelamination being delivered via buckling of the ﬁlm.The key mechanics ingredients of this mechanism havebeen presented by Marshall and Evans w4x, and Krieseand Gerberich w5x have recently extended the analysisto multilayer ﬁlms. On the other hand, coatings onrelatively ductile substrates often fail during indenta-tion by radial and in some cases circumferential cracksthrough the ﬁlm. The mechanics of delamination insuch systems has been analyzed by Drory and Hutchin-son w6x for deep indentation with depths that are two tothree orders of magnitude larger than the coatingthickness. The determination of interface toughness insystems that show coating cracking has been demon-strated recently by, e.g. Wang et al. w7x. In both types ofmaterial systems there have been reports of‘ﬁngerprints’ on the load displacement curves in theform of kinks w5,8,9x, in addition to the reduction ofhardness Žsoftening. envisaged in w2x. The origin of Fig. 1. Illustration of the boundary value problem analyzed in thisthese kinks remains somewhat unclear, however. study. A ﬁnal class considered in w2x is that of hard, strongcoatings on ductile substrates, where Swain and Mencik ˇhypothesized that indentation with a spherical indenter 2. Problem formulationwould not lead to cracking of the coating but just todelamination. This class has not yet received much 2.1. Go¨ erning equationsattention, probably because most deposited coatings,except diamond or diamond-like carbon, are not sufﬁ-ciently strong to remain intact until delamination. On We consider a system comprising an elastic per-the other hand, it provides a relatively simple system fectly plastic material Žsubstrate . coated by an elasticthat serves well to gain a deep understanding of the thin ﬁlm and indented by a spherical indenter. Thecoupling between interfacial delamination and plastic- indenter is assumed rigid and only characterized by itsity in the substrate. An analysis of this class is the radius R. Assuming both coating and substrate to besubject of this paper. isotropic, the problem is axisymmetric, with radial coor- In the present study, we perform a numerical simula- dinate r and axial coordinate z in the indentationtion of the process of indentation of thin elastic ﬁlm on direction, as illustrated in Fig. 1. The ﬁlm is character-a relatively softer substrate with a small spherical in- ized by its thickness t and is bonded to the substrate bydenter. The indenter is assumed to be rigid, the ﬁlm is an interface, which will be speciﬁed in the next section. The substrate is taken to have a height of L y t andelastic and strong, and the substrate is elastic perfectly radius L, with L large enough so that the solution isplastic. The interface is modeled by a cohesive surface, independent of L and the substrate can be regarded aswhich allows to study initiation and propagation of a half space.delamination during the indentation process. Separate The analysis is carried out numerically using a ﬁnitecriteria for delamination growth are not needed in this strain, ﬁnite element method. It uses a Total La-way. The aim of this study is to investigate the possibil- grangian formulation in which equilibrium is expressedity and the phenomenology of interfacial delamination. in terms of the principle of virtual work asOnce we have established the critical conditions fordelamination to occur, we can address more design-likequestions, such as what is the interface strength needed H ij i j d¨ q HS T dS s Ht i u i d s. Ž1.to avoid delamination. We will also study the ¨ i ¨‘ﬁngerprint’ left on the load displacement curve bydelamination, and see if delamination itself can lead to Here, ¨ is the total L = L region analyzed and ¨ iskinks as mentioned above in other systems. It is em- its boundary, both in the undeformed conﬁguration.phasized that the calculations assume that other failure With x i s Ž r, z, . the coordinates in the undeformedevents, mainly through-thickness coating cracks, do not conﬁguration, u i and t i are the components of dis-occur. placement and traction vector, respectively; i j are the
A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 145components of Second Piola Kirchhoff stress while i j rial with plastic ﬂow being controlled by the von Misesare the dual Lagrangian strain components. The latter stress. For numerical convenience, however, we adopt aare expressed in terms of the displacement ﬁelds in the rate-sensitive version of this model, expressed bystandard manner, n si j e ˙ ipj s 3r2 ˙ p , ˙ p s˙y ž / Ž7. i j s 1r2 u i , j q u j,i q u ,i u k , j k Ž2. Ž . e ywhere a comma denotes Žcovariant. differentiation with for the plastic part of the strain rate, ˙ ipj s ˙ i j y ˙ ej . irespect to x i. The second term in the left-hand side is Here e s 3r2 si j s i j is the von Mises stress, expressed the contribution of the interface, which is here mea- in terms of the deviatoric stress components si j , n issured in the deformed conﬁguration Ž Si s Ä zs t 4.. The the rate sensitivity exponent and ˙ y is a referenceŽtrue. traction transmitted across the interface has strain rate. In the limit of n ª , this constitutivecomponents T , while the displacement jump is , model reduces to the rate-independent von Mises plas-with being either the local normal direction Ž s n. ticity with yield stress y . Values of n on the order ofor the tangential direction Ž s t . in the Ž r, z . plane. 100 are frequently used for metals Žsee e.g. w10x., soHere, and in the remainder, the axisymmetry of the that the value of e , at yield is within a few percent ofproblem is exploited, so that u 3 s t 3 s i3 s i3 s 0. e y . The elastic part of the strain rate, ˙ i j , is given in The precise boundary conditions are illustrated in terms of the Jaumann stress rate asFig. 1. The indentation process is performed incremen-tally with a constant indentation rate ˙ Outside the h.contact area with radius a in the reference conﬁgura- ij s R i jk l ˙ e l k Ž8.tion, the ﬁlm surface is stress free, with the elastic modulus tensor R i jk l being determinedt r Ž r ,0. s t z Ž r ,0. s 0 for aF r F L. Ž3. by the Young modulus Es and Poisson’s ration s , Žsubscript s for substrate .. Inside the contact area we assume perfect sticking The coating is assumed to be a strong, perfectlyconditions so that the displacement rates are controlled elastic material with Young’s modulus E f and Poisson’sby the motion of the indenter, i.e. ration f Žsubscript f for ﬁlm.. The above equations, supplemented with the consti-u z Ž r ,0. s ˙˙ h, u r Ž r ,0. s 0 for 0 F r F a. ˙ Ž4. tutive law for the interface to be discussed presently, form a non-linear problem that is solved in a linear Numerical experiments using perfect sliding condi- incremental manner. For this purpose, the incrementaltions instead have shown that the precise boundary virtual work statement is furnished with an equilibriumconditions only have a signiﬁcant effect very close to correction to avoid drifting from the true equilibriumthe contact area and do not alter the results for de- path. Time integration is performed using the forwardlamination to be presented later. The indentation force gradient version of the viscoplastic law Ž7. due toF is computed from the tractions in the contact region, Peirce et al. w11x. aFs H0 t zŽ r ,0. 2 r d r . Ž5. 2.2. The cohesi¨ e surface model In the description of the interface as a cohesive The substrate is simply supported at the bottom, so surface, a small displacement jump between the ﬁlmthat the remaining boundary conditions read and substrate is allowed, with normal and tangential u z Ž r , L . s 0 for 0 F r F L; components n , and t , respectively. The interfacial Ž6. behaviour is speciﬁed in terms of a constitutive equa- u r Ž 0, z . s 0 for 0 F zF L. tion for the corresponding traction components Tn and Tt at the same location. The constitutive law we adopt However the size L will be chosen large enough that in this study is an elastic one, so that any energythe solution is independent from the precise remote dissipation associated with separation is ignored. Thus,conditions. it can be speciﬁed through a potential, i.e. The Eqs. Ž1. and Ž2. need to be supplemented withthe constitutive equations for the coating and the sub-strate, as well as the interface. As the latter are central T sy Ž s n,t . . Ž9.to the results of this study, these will be explained indetail in the forthcoming section. The substrate is The potential reﬂects the physics of the adhesionsupposed to be a standard isotropic elastoplastic mate- between the coating and substrate. Here, we use the
146 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154potential that was given by Xu and Needleman w12x,i.e. 1yq s nq n exp ž y n n /½ 1yrq n n ry1 ryq 2 y qq ž ry1 / n n exp y ž /52 t t Ž 10 .with n and t the normal and tangential works ofseparation (q s tr n ., n and t two characteristiclengths, and r a parameter that governs the couplingbetween normal and tangential separation. The corre-sponding traction separation laws from Eq. Ž9. read 2Tn s n n exp y ž n n /½ n ž / n exp y 2 t t 1yq 2 q ry1 1 y exp y ž / 5 2 t t ry n n ; Ž 11 .Tt s 2 n n ž / ½ n t t t qq ž rr y q / y1 n n 5 ž exp y n n / exp 2 t = y ž / 2 t . Ž 12. The form of the normal response, Tn s TnŽ t s 0. ismotivated by the universal binding law of Rose et al.w13x. In the presence of tangential separation, t / 0,Eq. Ž11. is a phenomenological extension of this law,while the tangential response Eq. Ž12. should be con- Fig. 2. The uncoupled normal and tangential responses according to the cohesive surface law Eqs. Ž11. and Ž12.. Ža. Normal responsesidered as entirely phenomenological. The uncoupled TnŽ n . with t s 0. Žb. Tangential response Tt Ž t . with n s 0. Bothresponses, i.e. with t s 0 Ž n s 0. for the normal are normalized by their respective peak values, ma x and max .Žtangential . response, are shown in Fig. 2. Both arehighly non-linear with a distinction maximum of thenormal Žtangential . traction of max Ž max . which occurs The coupling parameter r can be interpreted as theat a separation of n s n Ž t s t r 62.. The normal value of the normal separation nr n after completeŽtangential . work of separation, n Ž t ., can now be shear separation Ž tr t ª . with Tn s 0. Some insightexpressed in terms of the corresponding strengths max into the coupling between normal and shear responseŽ max . as can be obtained from Fig. 3, which shows the maximum shear traction as a function of the normal displace- n s exp ts 1r2expŽ1. ment, i.e. Ttmax Ž n . Tt Ž tr t s 1r 2 , n .. It is seen Ž1. max n, max t. Ž 13. that this is quite sensitive to the values of r and q. The Using Eq. Ž13. together with the relation q s tr n , maximum shear traction that can be transmitted de-we can relate the uncoupled normal and shear strengths creases when there is opening in the normal directionthrough Ž n ) 0. for all parameter combinations shown. How- ever, in normal compression Ž n - 0., the maximum 1 shear stress can either increase or decrease with y n . t max s max Ž 14 . An increase appears to be the most realistic, and the q 2exp Ž 1 . n parameter values used in the present study ensure this.
A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 147 interfacial shear strength maxr y on the initiation and advance of interfacial delamination. The relation between normal and tangential interfacial strengths is given by Eq. Ž14.. Three values of y r Es , were chosen, namely 0.0025, 0.005 and 0.01. For each value of y r Es , several values of max r y are chosen. Even though the solution is formally governed by the above-mentioned non-dimensional groups, we have chosen to work primarily in terms of real dimensional values in order to simplify the interpretation. We have used an indenter of radius R s 0.05 mm and a ﬁlm thickness t s 0.005 mm. The elastic properties are E f s 500 GPa, f s 0.33, Es s 200 GPa and s s 0.33. The yield stress of the substrate is varied, as discussed above, and the reference strain rate is taken to be ˙ y s 0.1 sy1 with n s 100. The indentation is per- formed under a constant rate ˙ s 1 mmrs. For a hFig. 3. The maximum shear traction Ttma x , normalized by max Žsee typical value of y r Es of 0.005, the value of the factorFig. 2., as a function of the normal separation for different combina- Ž t ˙ y Esr y ˙.1rŽ ny1. in Eq. Ž18. is 0.977; this is less than htions of the coefﬁcients r and q. In Ža. Žc., r s 0.5 2.5% smaller than the rate-independent limit. For the cohesive surface we have chosen the same values for y43. Results and discussion n , and t , namely 10 mm. Most of the results to be presented are for r s 0.5 and q s 0.5, but we will also3.1. Analysis and parameters brieﬂy investigate the sensitivity of the results to these values. As mentioned above, various values of max will The solution to the problem depends on a number of be considered; it should be noted that by using anon-dimensional parameters. We have chosen the fol- constant ratio q, the normal strength max varies with max according to Eq. 14 . The values of max to belowing non-dimensional groups: Ž . investigated vary between 0.3 and 1.4 GPa. This corre- R sponds to interfacial energies for shear failure ranginggeometry: Ž 15. from 35 to 160 Jrm2 which are realistic values for the t interface toughnesses for well-adhering deposited ﬁlms w3x. Ef ymaterial: , , f , c Ž 16 . The size L of the system analyzed ŽFig. 1. is taken to Es Es be 10 R. This proved to be large enough that the results are independent of L and therefore identical to those n n max for a coated half-inﬁnite medium. The mesh is aninterface : q, , , , r Ž 17 . arrangement of 19 600 quadrilateral elements, and t t y 21 291 nodes. The elements are built up of four linear strain triangles in a cross arrangement to minimize 1r Ž ny1 . t ˙ y Es numerical problems due to plastic incompressibility. To h Floading: , t R2 y ž / ˙ yh Ž 18. account properly for the high stress gradients under the indenter and for an accurate detection of the contact nodes, the mesh is made very ﬁne locally near the Note that the rather complex form of the last loading contact area with an element size of tr10.parameter is dictated by the fact that rate-dependent Consistent with the type of elements in the coatingplasticity, Eq. Ž7., is governed by the parameters ˙ y and and the substrate, linear two-noded elements are used y only through the combination ˙ y r y . This non-di- n along the interface. Integration of the cohesive surfacemensional parameter immediately shows that the in- contribution in Eq. Ž1. is carried out using two-pointdentation force depends on the indentation rate in a Gauss integration. Failure, or delamination, of the in-rate-dependent material. However, in the limit that terface at any location develops when exceeds .n ª , the bracketed factor becomes 1, so that the The critical instant is here taken to be when s .parameter reduces to FrŽ R 2 y .. Larger critical values may be used as well w14x, but In the results to be presented we focus mainly on the using two or three times does not signiﬁcantlyeffect of the normalized substrate yield strength yrEs , change the critical indentation depth or force.which is simply the yield strain, and the normalized The maximum indentation depth applied in all calcu-
148 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154lations is h max s 2 t. Further indentation can be done, behaviour. Note that the radial position r is normal-but was not considered relevant since real coatings will ized, for each h, by the current contact radius a.have cracked by then and the present model is no In the contact area below the indenter Ž r F a. thelonger applicable. interface is of course under high compression ŽFig. 4a.. The reason for this stress being the same for all inden-3.2. Perfect interface tation depths shown is that the contact region is con- tained within the plastic zone in the substrate, which exhibits no hardening. For r ) 3a roughly, there is an For the purpose of reference, we ﬁrst consider a annular region with an opening normal stress. Accord-coated system with a perfect interface, which would ing to Fig. 4b there are three regions in which thecorrespond to taking max r y ª . We have analyzed interfacial shear stress exhibits a local maximum Žinthis simply by rigidly connecting the coating to the absolute value.: near the edge of the contact radius, atsubstrate Žcf. also w15,16x.. Of particular relevance here, approximately 2 a and in a region between 3a and 5a.is the stress distribution that develops at the The highest shear stress, roughly 0.6 y , is attained incoating substrate interface. Fig. 4 shows the normal this outer region. Closer examination of the resultsŽ n . and shear Ž t . stress components at different reveals that this shear stress is caused by the outwardindentation depths for the case of yrEs s 0.0025. radial plastic ﬂow of the substrate under the indenterOther values of yrEs would give the same qualitative relative to the coating. The latter is being pulled in- wards due to the indentation. This relative motion is opposite to that observed in the calculations of Narasimhan and Biswas w17x who considered a plasti- cally deforming ﬁlm on a rigid substrate. The most noteworthy part of the stress distributions in Fig. 4 is that there is an annular region around r ) 3a where the shear stresses are larger and the normal stress is positive. This is relevant for delamina- tion because of the coupling between normal and tan- gential response of the interface. Rephrased in terms of the cohesive surface model used here, the opening normal stress, corresponding to n ) 0, signiﬁcantly reduces the maximal shear stress before shear failure, as shown in Fig. 3, so that this region r ) 3a is a potential location for delamination. 3.3. Initiation of delamination In the presence of cohesive surface along the inter- face, a distribution of normal and tangential separa- tions develops, Ž r ., with progressive indentation h. The actual initiation of delamination is identiﬁed when n r s n or t r s t for any r. The indentation Ž . Ž . depth at this instant is denoted by h c , the correspond- ing contact radius is a c and the critical position is rc . For all parameter combinations investigated Žcf. Sec- tion 3.1. we indeed ﬁnd that delamination occurs by tangential failure, t Ž r . G t . A parameter study has been carried out to determine the dependence of h c , rc and a c on the two key material characteristics: the substrate yield strength y and the interfacial shear strength max . This is done by scanning, for three values of yrEs , several values of the ratio max r y . In the case of yrEs s 0.0025, theFig. 4. Interfacial tractions along a perfectly bonded interface at values of max r y are 0.6, 0.7, 0.75, 0.8, 0.85 and 0.86,three indentation depths Ž a is the instantaneous contact radius. for in the case of yrEs s 0.005 the values are 0.3, 0.4, 0.5, y rEs s 0.0025. a Normal stress. b Shear stress. Ž . Ž . 0.6, 0.7, 0.75 and 0.8, and in the case of yrEs s 0.01
A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 149the values are 0.2, 0.3, 0.4, 0.5, 0.6 and 0.7. For each y rEs , higher values of max r y were considered butabove a certain value delamination was not found. Thefact that there is a limiting value for the interfacialstrength above which delamination is prevented will bediscussed in the next subsection. Fig. 5 summarizes the obtained values of h c , rc , anda c , for the various cases. Fig. 5a shows that for each ofthe three substrate yield strengths, rc increases withthe interface strength max r y in proportion with theindentation depth h c . It should be noted that the directproportionality between rc and h c is valid for the rangeof interface stresses considered here, but breaks downat much smaller strengths. The strengths consideredhere are such that the indentation depth has to reachroughly the coating thickness t before delamination Fig. 6. Ža. Critical indentation depth h crt and Žb. critical delamina- tion radius rcrR vs. relative interfacial strength maxr y. Discrete points are results from the numerical computations; the lines are according to ﬁts: Ža. Eq. Ž21.; Žb. Eq. Ž22.. occurs. The radius at which delamination then initiates is seen to be on the order of the indenter radius R which here is 10 t. Fig. 5b shows that this delamination radius is between two and four times the contact radius a, this factor depending on both interface strength and substrate yield strength. For yrEs s 0.0025, we ﬁnd rcrR ) 3a crR, which is consistent with the expectation in the previous section. The same data are re-plotted in Fig. 6 but now as a function of the ratio between interface and substrate yield strength. We see that both h c and rc increase non-linearly with maxr y . Contrary to rc , which ap-Fig. 5. Ža. Location of delamination initiation rc vs. critical indenta- pears to be depending practically only on maxr y ŽFig.tion depth h c . Žb. rc vs. contact radius at delamination initiation.Discrete points are results from the numerical computations; the 6b., the indentation depth h c , is quite a strong functionlines are Ža. linear Žsee Eq. Ž19.. and Žb. second degree polynomial of the substrate yield strain ŽFig. 6a.. The latter stronglyﬁts. The arrows indicate the direction of increasing ma xr y . indicates that plastic deformation in the substrate is a
150 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154key factor in determining whether or not delaminationtakes place Žwe will return to this later.. The results presented in Fig. 5 can be ﬁtted quiteaccurately by the following relationships:rcrRs a1Ž h crt . q a2 , Ž 19 .Ž max r y .Ž rcrR . 2 s a3 Ž h crt . q a4 , Ž 20. The least squares method has been used to obtainthe coefﬁcients a1 , through a4 for the best ﬁt for eachof the three values of yrEs Žsee Table 1.. The rela-tionships Ž19. and Ž20. can be combined to giveŽ max r y .Ž a1Ž h crt . q a2 . 2 s a3 Ž h crt . q a4 , Ž 21. Fig. 7. Evolution with indentation depth h of shear stress t , normal 2 opening n and corresponding peak tangential traction Ttma x Ž n . at max r ya1Ž .Ž rcrR . s a3 Ž rcrRy a2 . q a1 a4 , Ž 22. r s 1.24R.which have then been plotted in Fig. 6. It is seen thatthey give a reasonable representation to the numerical be attributed to the coupling in the interface behaviourresults over the range of parameters considered here. as described by Eqs. Ž11. and Ž12..As mentioned before, the critical indentation depth In the presence of coupling, the maximal tangentialdiffers from the trend in Fig. 5 for much smaller values traction Ttmax at any point along the interface dependsof the interface strength so that extreme care must be on the local normal displacement n , as shown in Fig.taken by extrapolation of Eqs. Ž19. Ž22. outside the 3. The interfacial region that is of interest then isconsidered parameter range. r ) 3a or so, where a tensile interface stress develops during indentation ŽFig. 4a., since the corresponding3.4. Strength limit to delamination normal opening of the cohesive surface reduces the local shear strength Ttmax . Fig. 7 demonstrates this As mentioned before, there is value of max r y coupling for the case yrEs s 0.0025 and maxr y sbeyond which delamination does not take place. This 0.87, for which delamination did not occur. This ﬁgurevalue is seen in Fig. 6 to be dependent on yrEs and, shows the evolution of n , t and Ttmax Ž n . with inden-upon closer examination, is related to the coupling tation depth at r s 1.24R Žthis is the location wherebetween normal and tangential behaviour of the inter- delamination does initiate when maxr y s 0.86.. Weface. In the absence of this coupling, the shear stress see that the local shear stress at the interface graduallyalong the interface is limited by the plastic ﬂow in the increases to a value of approximately yr63, whichsubstrate. In the time-independent limit, n ª in Eq.Ž7., we have e F y so that the maximum value that evidences that the plastic zone gradually engulfs thisthe shear stress can reach at the interface is yr63; point. As this occurs, n , increases until a certainwhen plasticity is slightly rate-dependent as here Ž n s indentation depth and the effective shear strength Ttmax100. this value can be somewhat larger but yr63 is decreases. However, just before Ttmax would coincidestill a very good estimate. Hence, if the interface re- with t and delamination would initiate, the normalsponse is not coupled, delamination is not possible for opening starts to decrease and delamination becomesstrengths max exceeding yr63. The reason for which excluded.we ﬁnd delamination in Fig. 6 at higher maxr y must Fig. 8 summarizes the limiting values of the interfa- cial shear strength max for the various cases analyzedTable 1 and plots them directly vs. the substrate yield strength.Coefﬁcients for ﬁtting relations Eqs. Ž19. Ž22. There appears to be a rather good linear correlation over the range considered, with the deviation from the y r Es a1 a2 a3 a4 line yr63 increasing with y . The ﬁgure also shows0.0025 1.3072 y0.6828 0.5799 0.3497 the two values for interfaces characterized by different0.005 0.8863 y0.5610 0.3672 0.4377 values of q s tr n than 0.5, namely q s 0.3 and 0.7.0.01 0.5403 y0.4316 0.2298 0.4954 According to Fig. 3, a smaller value of q, for example,
A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 151 constant steady-state speed after traveling a certain distance from the initiation point. The reason for this is that the dominant driving force for initial propagation is the elastic energy stored in the system; once this energy gets released, it gives rise to more or less instantaneous growth which is just limited here by the rate at which plastic deformation can evolve in the substrate. On the other hand, the steady state propaga- tion is predominantly driven by the indentation process which is performed at a constant rate, thus explaining the constant steady-state propagation speed. It is of interest to mention here that for some parameter combinations, such as yrEs s 0.01 and max r y s 0.7, we encounter numerical instabilities af- ter the onset of delamination. We attribute this to the stored elastic energy in these cases being so large that ellipticity of the problem is locally lost when this energyFig. 8. The interfacial shear strength ma x above which delaminationis excluded as a function of the substrate yield stress y . Open circlesare the numerical results, while the solid line is a linear ﬁt Žthedash-dotted line is the limit in the absence of coupling betweennormal and tangential separation in the interface .. The symbols qand U represent isolated results for q s 0.3 and q s 0.7, respectively.implies a stronger reduction of the interfacial shearstrength. Hence, the smaller q, the larger the value of max that suppresses shear delamination. It is seen fromFig. 8 that the result is quite sensitive to the precisevalue of q.3.5. Propagation of delamination After delamination initiates at the location rc and ata corresponding indentation depth h c , it propagates asa shear crack in both directions: towards and awayfrom the indenter. The tip of the zone that propagatestowards the indenter gets arrested after a short timebecause of the compressive normal traction close to thecontact area as seen in Fig. 4a. The leading tip of thedelaminated zone keeps propagating with continuedindentation. Fig. 9a shows the leading tip location,r frR, as a function of the indentation depth, hrt, forthe case of yrEs s 0.0025 Žother values of yrEs showthe same qualitative behaviour., and for four differentvalues of interfacial strength. The width of the ring-shaped delaminated area, Ž r f y ri .rR, is shown in Fig.9b as a function of the indentation depth. Since theindentation rate ˙ is constant, the propagation speed ˙f h rcan be expressed as given by R Ž r frR .˙f s ˙ tr h Ž hrt . Fig. 9. Ža. Location of the leading tip of the delaminated zone, r f , vs.so that it is simply ˙Ž Rrt . times the slope of the curves h indentation depth h. Žb. The width of the ring-shaped delaminatedin Fig. 9a. In each of the four cases shown, delamina- zone, r f y ri , vs. indentation depth h. This ﬁgure is for the case oftion starts off with a relatively high speed and reaches a y r Es s 0.0025, and several values of interfacial strengths.
152 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154is released. More advanced solution procedures arenecessary to handle this. To further demonstrate the interaction between de-lamination and plasticity in the substrate, Fig. 10 showsthe distribution of the Von Mises effective stress e inthe indented region for hrt s 1.5. The particular caseshown is for maxr y s 0.8 and yrEs s 0.0025. For thepurpose of comparison, the distribution for the case ofa perfectly bonded interface is included as well wFig.10ax. The region in the substrate where the value of eis close to y signiﬁes the region of substantial plastic Fig. 11. Normalized load vs. indentation depth curves for different values of y r Es . Dashed lines represent cases with perfect interface and solid lines represent cases with a ﬁnite-strength interface with ma x r y s 0.6. The dash-dotted lines identify the initiation values h s h c , Žcf. Fig. 6a.. deformation Žnote that we are using viscoplasticity so that e is not limited to y .. The delaminated zone in Fig. 10b is identiﬁed by a white line, and extends from ri f 0.04 mm to r f f 0.07 mm. It initiated at an indenta- tion depth of h c r t s 1.16 and a critical radius of rc f 0.05 mm. Comparison of the two plots shows, ﬁrst of all, that a plastic region has developed near the leading tip of this zone with a size on the order of the coating thickness. This plastic zone moves with the propagating tip of the delamination zone. Apparently, there is a stress concentration around the tip of the delaminated zone which induces local plastic ﬂow in the substrate. The second difference between Fig. 10a and b is that a perfectly bonded interface induces a plastic zone in the substrate that is somewhat larger than in the case of a ﬁnite-strength interface. This is attributed to the fact that interfacial delamination serves as another mecha- nism for stress relaxation in the system. Except for the near-tip region of the delaminated zone, this tends to reduce the necessity for stress relaxation by plastic deformation, thereby reducing the overall dimension of the plastic zone. 3.6. Load ¨ s. depth of indentation One of the most common outputs of indentation experiments is the indentation force vs. indentation depth curve Žload displacement curve.. Fig. 11 shows the predictions for some of the cases considered hereFig. 10. Contours of the Von Mises effective stress at hrt s 1.5 for with an interface strength of maxr y s 0.6, in compar- y r Es s 0.0025. a Perfectly bonded interface; b ﬁnite-strength Ž . Ž .interface with ma xr y s 0.8. The white line in Žb. denotes the ison with the corresponding ones for the perfect inter-delaminated zone, the arrows indicating the direction of interfacial face. Prior to initiation of delamination, the resultsshear. differ very slightly from those with a perfectly bonded
A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 153coating, which is just due to the ﬁnite stiffness of the In all cases analyzed, delamination initiates at acohesive surface. After initiation of the shear delami- radial location that is more than twice the contactnation, h ) h c , the system is noticeably more compli- radius, and propagates in two directions; towards andant, yielding an indentation force that is reduced by away from the indenter, thus generating a ring-shapedbetween 5 and 10% compared to the same case with delaminated zone. The front which travels towards thethe perfect interface. indenter gets arrested after a short distance because of For the smaller yield strengths, the effect of delami- the compressive normal stress in that region. After anation in the F h curve evolves gradually, but a dis- high initial speed of propagation, the other top settlestinct kink at h s h c is observed in Fig. 11 for yrEs s at a steady propagation at a constant velocity. The0.01. Similar kinks have been observed experimentally initial propagation speed is governed by the high elasticby Hainsworth et al. w8x and Li and Bhuchan w9x, but energy stored in the system prior to delamination,they have been associated with through-thickness ring while the steady-state speed is controlled by the inden-or radial cracks. The kink found here is a result of the tation process itself.high energy release rate at the moment of crack initia- It bears emphasis at this point to recall that thetion, that gives rise to almost instantaneous growth of coating is assumed to be elastic and strong. Deviationsthe delaminated zone Žsee Fig. 9a.. Since the amount from this, such as plasticity of the coating or cracking,of stored elastic energy is higher for higher interfacial may affect our ﬁndings both for the initiation and thestrength and higher substrate yield stress, the kink will propagation of delamination. As mentioned in Sectionbe sharper accordingly. 1, cracking is a potential mechanism for hard coatings and will change the picture dramatically; this requires a totally different analysis. However, plastic deformation4. Conclusions in the hard coatings under consideration will be limited to plastic zones immediately under the indenter, which Numerical simulations have been carried out of the are often smaller than that in the substrate. In suchindentation process of a coated material by a spherical cases, the precise instant of delamination and the rateindenter. The interface between the ﬁlm and the sub- of propagation are expected to differ somewhat quanti-strate was modeled by a cohesive surface, with a cou- tatively, but to leave the phenomenology essentiallypled constitutive law for the normal and the tangential unchanged.response. Failure of the interface by normal or tangen- For simplicity, the present calculations have assumedtial separation, or a combination, is embedded in the perfect but rate-dependent plasticity for the substrate.constitutive model and does not require any additional Rate dependency was never signiﬁcantly affecting thecriteria. results here because the time scale for the indentation A parametric study has been carried out to investi- process was always much larger. Strain hardening ofgate the inﬂuence of interfacial strength and substrate the substrate will, obviously, change the quantitativeyield strength on delamination. Delamination is found results, especially for the indentation force vs. depthto be driven by the shear stress at the interface associ- response. However, we do not expect a qualitativelyated with the plastic deformation in the substrate, and signiﬁcant effect on delamination, since the leadingconsequently occurs in a tangential mode. Neverthe- front of the delaminated zone seems to propagate withless, interfacial normal stresses have a signiﬁcant effect the front of the plastic zone in which hardening has noton delamination, due to the coupling between normal yet taken place.and tangential response. Here we have focused on the Again for simplicity, this study has not accounted forcoupling whereby the interfacial resistance to tangen- the presence of residual stress in the coating, due fortial delamination is reduced by tensile stresses along example to thermal mismatch relative to the substrate.the interface. This as well as the inﬂuence of wavy interfaces will be We ﬁnd, however, that the results are quite sensitive examined in a forthcoming paper.to variations in this coupling so that quantitative pre-dictions require an accurate description of this inter- Referencesface coupling. This pertains, for instance, to the valueof the interfacial shear strength above which delamina- w1x T.F. Page, S.V. Hainsworth, Surf. Coat. Technol. 61 Ž1993. 201.tion never occurs. In the absence of any coupling w2x ˇ M.V. Swain, J. Mencik, Thin Solid Films 253 Ž1994. 204.between normal and tangential response, this limiting w3x A. Bagchi, A.G. Evans, Interface Sci. 3 Ž1996. 169.strength is simply max s yr63, but it is signiﬁcantly w4x B.D. Marshall, A.G. Evans, J. Appl. Phys. 56 Ž1984. 2632. w5x M.D. Kriese, W.W. Gerberich, J. Mater. Res. 14 Ž1999. 3019.higher due to the coupling. This indicates that espe- w6x M.D. Drory, J.W. Hutchinson, Proc. R. Soc. London A 452cially this coupling in the adopted interface model Eqs. Ž1996. 2319.Ž11. and Ž12. needs closer examination and comparison w7x J.S. Wang, Y. Sugimora, A.G. Evans, W.K. Tredway, Thin Solidwith dedicated experiments. Films 325 Ž1998. 163.
154 A. Abdul-Baqi, E. Van der Giessen r Thin Solid Films 381 (2001) 143 154 w8x S.V. Hainsworth, M.R. McGurk, T.F. Page, Surf. Coat. Tech- w13x J.H. Rose, J. Ferrante, Phys. Rev. Lett. 47 Ž1981. 675. nol. 102 Ž1997. 97. w14x X.-P. Xu, A. Needleman, J. Mech. Phys. Solids 42 Ž1994. 1397. w9x X. Li, B. Bhushan, Thin Solid Films 315 Ž1997. 214. w15x M.R. Begley, A.G. Evans, J.W. Hutchinson, Int. J. Solids Struct.w10x R. Becker, A. Needleman, O. Richmond, V. Tvergaard, J. 36 Ž1999. 2773. Mech. Phys. Solids 36 Ž1988. 317. w16x S. Sen, B. Aksakal, A. Ozel, Int. J. Mech. Sci. 40 Ž1998. 1281.w11x D. Peirce, C.F. Shih, A. Needleman, Comput. Struct. 18 Ž1984. w17x R. Narasimhan, S.K. Biswas, Int. J. Mech. Sci. 40 Ž1997. 357. 875.w12x X.-P. Xu, A. Needleman, Model. Simul. Mater. Sci. Eng. 1 Ž1993. 111.